Polymer defect engineering – conductive 2D organic platelets from precise thiophene-doped polyethylene

Synthesis and crystallization of polyethylene with precisely positioned thiophene groups were used to produce polymer crystals with a conductive surface.


Introduction
Conductive polymers combine the mechanical advantages of polymers with the electronic properties of metals and semiconductors, which makes them valuable in the electronics and optical industries. [1][2][3] Some of the most common organic molecules to obtain conductive materials are thiophene and its derivatives, because of their good electrical and chemical properties and environmental stability (both to oxygen and to moisture). 4 However, the conjugated backbone of un-substituted polythiophenes is typically rigid and results in poor processability. 5 To obtain control over the nanostructure and to increase the processability of thiophene containing materials, two different approaches have been described in the literature: the first approach utilizes the self-assembly of a polymer system to form a nanoscopic template. 6 Subsequently, a conductive polymer like polythiophene is grafted upon this template. The resulting nanostructures thus formed have a dielectric core, but the surfaces show only a partial conductivity. The other approach aims to generate a polymeric material with bulk conductivity first. 7 Subsequently, this conductive polymer is attached to a dielectric layer, which involves several additional steps.
Here, we demonstrate a unique method to generate 2D polymer nanoplatelets with conductive surfaces. To achieve this, we utilize the crystallization driven self-assembly of a precisely synthesized polyethylene-based polymer with in-chain thiophene groups. We use acyclic diene metathesis (ADMET) polymerization 8 to synthesize the necessary polymer. This approach allows us to generate an equidistant distribution of functional groups along the polymer backbone. 9, 10 We designed the polymer architecture in a way, so that the crystallization of this polymer automatically yields the desired 2D nanoplatelets with the thiophene groups arranged exclusively on their surface. Although the thiophene groups are arranged with crystal perfection on the surface, their intramolecular distance is too large to allow for charge carrier transport. Hence, to achieve the final surface conductivity of these nanoplatelets, we copolymerize the surface protruding thiophene groups with 3,4-ethylenedioxythiophene (EDOT). The resulting 2D nano platelets thus designed show a significant increase of conductivity after this copolymerization.

Instrumentation
Thin layer chromatography (TLC) was performed using Merck aluminium-foil baked plates coated with Kieselgel 60 F245. The products were visualized using UV fluorescence (254 nm) or potassium permanganate stain. Flash column chromatography was performed over Merck silica gel C60 (40-60 μm) using eluent systems as described for each experiment. 1  Mass spectrum acquisitions were conducted on an Advion expression L compact mass spectrometer (CMS) by using the atmospheric solid analysis probe (ASAP) technique. All spectra were acquired in the positive ion reflectron mode, m/z range from 10 to 2000 m/z, and acquisition speed 10 000 m/z units per s. The obtained spectra were analyzed by using Advion CheMS Express software version 5.1.0.2.
Gel-permeation chromatography (GPC) measurements were carried out in THF, with 1 g L −1 sample concentration. Sample injection was performed using a 717 plus auto sampler (Waters) at 30°C (THF). Flow was 1 mL min −1 . Three SDV columns (PSS) with the dimensions 300 × 80 mm, 10 μm particle size and pore sizes of 106, 104, and 500 Å were employed. Detection was accomplished with a DRI Shodex RI-101 detector (ERC) and a UV-vis S-3702 detector (Soma). Calibration was carried out using polystyrene standards provided by Polymer Standards Service. Thermal analysis by differential scanning calorimetry (DSC) was carried out using a Mettler-Toledo DSC 822. Three scanning cycles of heating/cooling were performed under a nitrogen atmosphere (30 mL min −1 ) with a heating and cooling rate of 10°C min −1 in a temperature range between −50 and 250°C for polymers TH20, TH20-H, TH38, TH38-H and between −120 and 250°C for all samples before and after oxidative coupling.
Thermal gravimetric analysis (TGA) was performed on a Mettler Toledo ThermoSTAR TGA/SDTA 851-Thermowaage under a nitrogen atmosphere. The heating rate was 10°C min −1 in a temperature range between 25 and 900°C.
For transmission electron microscopy (TEM) measurements, a FEI Tecnai F20 transmission electron microscope operated at an acceleration voltage of 200 kV was used to determine the crystal morphology and crystal structure. Bright field (BF) and parallel beam nano-electron diffraction (NBED) were used for measurements.
Conductivity measurement: glass substrates were sequentially cleaned with detergent, acetone, and 2-propanol by sonication for 5 min each and then dried. Polymers TH38-H, B and C (Scheme 2) were crystallized on the substrate from hot ethyl acetate, and dispersion of polymer A (Scheme 2) was applied on the substrate without additional preparation. Au electrodes were deposited on the dried films by thermal evaporation through shadow masks with a rate of 1 Å s −1 under a high vacuum of 10 −7 mbar. The spacing between the electrodes amounted to 20 µm, and the electrode width was 10 000 µm. Current (I)-voltage (V) measurement was performed using a Keithley 4200A semiconductor parameter analyzer in a vacuum probe station under 10 −5 mbar.

Synthesis of Grignard reagent and ADMET diene monomers TH20-m and TH38-m
All reactions have been carried out under an argon atmosphere. Into a flame-dried 25 mL 3-neck round-bottom flask, equipped with reflux and a tube with CaCl 2 on the top neck and connected with an argon line on the left neck, magnesium metal pellets were added (0.34 g, 14.2 mmol, 3.45 eq.) and then a magnetic stirrer was used. After 10 min, one iodine crystal and 10 mL of THF were added. The mixture was heated to 40°C and the first halide of the alkyl bromides, i.e. 11-bromo-1-undecene (1.49 mL, 6.8 mmol, 1.5 eq.) for TH20-m or 18-bromo-1-octadecene (2.25 g, 6.8 mmol, 1.5 eq.) for TH38m, was added. The reaction mixture slowly changed its color to dark blue, and then the second half of the respective alkyl halide was added. The mixture was allowed to stir until almost the whole magnesium metal pellets disappeared (ca. 30-40 min). After that, a solution of 3,4-dibromothiophene (1) (0.5 mL, 4.5 mmol, 1.0 eq.) in 10 mL THF was added, followed by (1,3-dppp)NiCl 2 (0.12 g, 0.2 mmol, 0.05 eq.). The reaction mixture was stirred at room temperature overnight and then poured into a mixture of water and hydrochloric acid. The aqueous layer was extracted with ether twice; combined organic phases were dried over anhydrous MgSO 4 , filtered and dried under reduced pressure.
The product was purified by column chromatography over silica gel eluting with petroleum ether to give 3 as a pale yellow oil. Yield 73% for TH20-m and 75% for TH38-m. 1  Procedure for ADMET bulk polycondensation of TH20 and TH38 Monomer TH20-m (0.7 g, 1.80 mmol, 1 eq.) or monomer TH38-m (0.6 g, 1.026 mmol, 1 eq.) was charged into a flamedried 25 mL flask in CH 2 Cl 2 (2 mL) and the solution was stirred for 5 min at room temperature under argon. Then, the 1st generation Grubbs catalyst (0.01 eq.) was added to this solution under an argon atmosphere. After the addition of the catalyst, the reaction mixture was stirred for 1 h at room temperature under argon flow and then evacuated to 5 × 10 −2 mbar for 2 h, at 40°C for 2 h, at 60°C for 5 h and at 80°C for 10 h to remove ethylene and remaining solvent. The reaction mixture was cooled to room temperature and the catalyst was terminated by adding ethyl vinyl ether (1 mL in 2 mL of CH 2 Cl 2 ), followed by 30 min stirring at room temperature. The reaction mixture was precipitated into methanol (100 mL). A brown, highly viscous polymer (4) was obtained after removal of the solvent in vacuo (Yield: 73%). 1 H NMR TH20

Hydrogenation of polymer TH20
The hydrogenation was performed using a 1st generation Grubbs catalyst modified with ethyl vinyl ether as the catalyst. 11 In a glass vessel, TH20 (500 mg) was dissolved in 10 mL THF and argon was bubbled through the solution for 5 min. Upon addition of the catalyst (1% mol), the solution changed its color to orange. The hydrogenation was performed in a 250 mL ROTH autoclave. The system was flushed twice with hydrogen; afterwards the hydrogenation was performed at 40°C and 70 bar H 2 for 2 days. The dark brown solution was concentrated in vacuo before precipitating into cold methanol to yield an off-white solid material (80% yield). 1

Hydrogenation of polymer TH38
The hydrogenation was performed using a 1st generation Grubbs catalyst modified with ethyl vinyl ether as the catalyst. In a glass vessel, TH38 (300 mg) was dissolved in 10 mL toluene and argon was bubbled through the solution for 5 min. Upon addition of the catalyst (1 mol%), the solution changed its color to orange. The hydrogenation was performed in a 250 mL Roth autoclave. The system was flushed twice with hydrogen; afterwards the hydrogenation was performed at 50°C and 65 bar H 2 overnight. The dark brown solution was concentrated in vacuo before precipitating into cold methanol to yield an off-white solid material (80% yield). 1

Oxidative coupling
All experiments were performed under an argon atmosphere.
In dispersion of nanoplatelets. FeCl 3 (0.11 g, 0.68 mmol, 4 eq.) was dissolved in 10 mL dry ethyl acetate and cooled to 0°C in an ice bath. TH38 (0.1 g, 0.17 mmol, 1 eq.) was dissolved in 5 mL ethyl acetate, heated up to 70°C and cooled down to room temperature within 30 min to form polymer platelets. The obtained dispersion was cooled to 0°C and added dropwise to the FeCl 3 solution. Subsequently, the mixture was stirred for 2 h at 0°C, then warmed up to room temperature and stirred for 24h and precipitated into 80 mL of methanol.
In solution. FeCl 3 (0.11 g, 0.68 mmol, 4 eq.) was dissolved in 10 mL dry CHCl 3 and cooled to 0°C in an ice bath. TH38 (0.1 g, 0.17 mmol, 1 eq.) was dissolved in 5 mL CHCl 3 , cooled to 0°C and added dropwise to the solution. This mixture was stirred for 2 h at 0°C, then warmed up to room temperature and stirred for 24 h and finally precipitated into 80 mL methanol.
In dispersion of nanoplatelets with EDOT. FeCl 3 (0.11 g, 0.68 mmol, 4 eq.) was dissolved in 10 mL dry ethyl acetate and solution was cooled down to 0°C in an ice bath. TH38 (0.1 g, 0.17 mmol, 1 eq.) was dissolved in 5 mL ethyl acetate, heated up to 70°C and slowly cooled down to room temperature to form polymer crystals. EDOT (0.04 mL, 0.37 mmol, 1.1 eq.) was added to the polymer crystal dispersion. The mixture was cooled to 0°C and added dropwise to the FeCl 3 solution. After several minutes, the color of the reaction mixture turned dark blue. The mixture was stirred for another 2 h at 0°C, then warmed up to room temperature and stirred for 24 h before precipitation in methanol.
Negative control experiment. FeCl 3 (0.11 g, 0.68 mmol, 4 eq.) was dissolved in 10 mL dry ethyl acetate and the solution was cooled down to 0°C in an ice bath. A structurally similar polyphosphoester 12 (0.11 g, 0.17 mmol, 1eq) was dissolved in 5 mL ethyl acetate, heated up to 70°C and slowly cooled down to room temperature to form polymer crystals. EDOT (0.04 mL, 0.37 mmol, 1.1 eq.) was added to the polymer crystal dis-

Results and discussion
Two polyethylene-like polymers carrying precisely spaced thiophene units were prepared by ADMET polymerization. The distance between the thiophene groups was adjusted to either 20 or 38 methylene units, which should influence the thermal properties of the resulting polymers. The monomers TH20-m and TH38-m for ADMET polymerization were prepared according to Scheme 1 in THF with an excess of 11-bromo-1-undecene or 18-bromo-1-octadecene, respectively. After column chromatography, the structure of TH20-m and TH38-m was confirmed by NMR and mass-spectroscopy ( Fig. S1 top, S2 top, S3 top, S4 top, Fig. S5 and S8 †). Peaks with masses 388.1 and 585.9 are responsible for di-substituted thiophene derivatives. The terminal olefin protons were detected at 4.9 and 5.7 ppm and the terminal olefin carbon signal at 139.3 and 114.1 ppm from 1 H and 13 C spectra, respectively, indicating that the alkylation reaction was successful. The ADMET polymerization of TH20-m and TH38-m was carried out in the bulk using 1% of the first generation Grubbs catalyst. Instead of terminal double bond multiplets at 4.9 and 5.7 ppm, a new internal double bond multiplet at 5.30 ppm was detected on 1 H spectra after ADMET polycondensation (Fig. S1 middle and Fig. S3 middle †). In the 13 C NMR spectra, the resonances of the terminal olefins vanished (Fig. S2 middle and Fig. S4 middle †) and a new signal at 130.4 ppm was detected, which was assigned to the internal double bonds of the polymer.
Internal double bonds in TH-20 and TH38 were hydrogenated in the presence of Grubbs catalyst 1st generation modified with ethyl vinyl ether as the catalyst. Structures of successfully hydrogenated polymers TH20-H and TH38-H were confirmed by NMR spectroscopy. Comparison of the polymers before and after hydrogenation reveals the disappearance of the double bond resonances at 5.30 ppm for 1 H spectra and at 130.4 ppm for 13 C NMR spectra, confirming successful hydrogenation of the polymers (Fig. S1, S2, S3 and S4 bottom †).
Molecular weights of TH20-H and TH38-H were determined by SEC in THF vs. polystyrene standards and were in accordance with the values of the respective unsaturated polymers (Fig. S6 and S9 †). The obtained TH20-H and TH38-H revealed an apparent molecular weight M w of ca. 23 400 g mol −1 (by SEC, M w /M n = 2.2) for TH20-H and 6300 g mol −1 (by SEC, M w /M n = 1.7) for TH38-H. Due to the low solubility of the sample with 38 CH 2 units, probably a lower degree of polymerization was achieved.

Solid state characterization
Both the non-hydrogenated and the hydrogenated polymers were able to crystallize, as shown by the DSC thermograms in Fig. 1 and S7. † The hydrogenation increased the melting temperature T m from −36 to 56°C for TH20 and from 50 to 77°C for TH38 as the internal cis-double bonds act as crystallization defects in the unsaturated polymer structures.
By elongating the aliphatic spacer between the thiophene units, the frequency of crystallization-defects is reduced, which resulted in increased melting temperatures. As the solution crystallization temperature of the TH20-H polymer was relatively low (39°C), the further oxidative coupling experiments were carried out exclusively with the TH38-H polymer.
The crystal structure of TH38-H lamellar crystals was determined by TEM and WAXS measurements. TEM measurement ( Fig. 2A) revealed crystals of truncated lozenge shape. The SAED diffraction pattern proved an orthorhombic structure, Scheme 1 Synthesis of thiophene diene monomers with different lengths of the aliphatic spacers and the ADMET polymerization and hydrogenation.

Paper
Polymer

Oxidative coupling
To achieve conductive properties, a covalent bond between thiophene groups is necessary to form a conjugated oligomer or polymer. 13 For the oxidative coupling of the initial polymer two distinct approaches were chosenin homogeneous solution or "on-surface" of the 2D nanoplatelets after they had been crystallized from a dilute solution. First, oxidative coupling in solution (Scheme 2A) was performed using anhydrous chloroform as a solvent. This experiment was necessary to check, whether the thiophene groups in the polymer backbone can react with each other despite their relatively low abundance. The polymer was completely soluble in chloroform and during the polymerization agglomeration occurred. After 24 h, a dispersion of black and almost insoluble polymer particles was obtained due to the intra-and intermolecular crosslinking of the thiophene units. Visualization of the dispersion via TEM proved the formation of particles with diameters of ca. 250 nm (Fig. S10B left †). The random crosslinking hinders the formation of continuous conductive layer. Therefore, the polymerized product did not show a significant increase in conductivity and probably only dimers or very short oligomers had been formed during the reaction (Fig. S10C left †). It is well known for thiophene polymers that during polymerization in solution the solubility drastically decreases which practically impedes processing and exploitation of the final product. 14 DSC measurement of the randomly cross-linked polymer (Fig. S10D left †) reveals only a minor glass transition temperature peak at 55°C, which is in good agreement with other polythiophene polymers. 15 Instead of utilizing the in-chain thiophene groups in solution, we crystallized the polymer prior to the thiophene polymerization from a dilute solution to prepare anisotropic polymer nanoplatelets with expelled thiophene units to their surface as previously proven for structurally similar polyphosphoesters. 12 Although the lamellar crystals are supposed to have the thiophene groups at their surface, they were non-conductive ( Fig. 3c left column). To achieve conductivity, the thiophene groups need to be covalently bonded, e.g. by polymerization on the crystal surface (Scheme 2).
For the polymerization of the thiophene groups on the crystal surface, we have to take care that the crystals are not destroyed, e.g. by melting or dissolution during the process. Hence, the oxidative polymerization of the thiophene groups was carried out in cold ethyl acetate, which allowed conserving the polymer crystals, in the presence of FeCl 3 as a catalyst (Scheme 2B). 16 After 24 h, the color of the dispersion turned light brown, which indicated the partial oxidation of FeCl 3 . The TEM measurement reveals that the TH-38 crystals stayed intact (Fig. S10B right †), but the electrical conductivity did not show a marked increase as compared to the initial nanoplatelets ( Fig. S10C right †). The lack of conductivity after reaction with FeCl 3 can be explained by the arrangement of the thiophene groups on the crystal surface. Assuming an orthorhombic crystal structure of the TH-38 (with lattice constants a = 7.5 Å and b = 5.1 Å), the minimal thiophene-to-thiophene distance is 9.1 Å (in (110) direction). Hence, several additional molecules may be necessary to bridge the thiophene units. Thus, it is likely that thiophene groups only react to a low extent in the amorphous parts but could not generate conjugated bonds on the surface of the crystals.
To covalently bond thiophene units on the crystal surface with each other, we added EDOT as a comonomer which Scheme 2 Reaction scheme of the oxidative coupling of TH-38H. The thiophene groups are expelled to the lateral surface of the lamellar polymer crystal. The distance between the thiophene groups is too large to allow charge transport. Accordingly, the thiophene groups need to be polymerized to achieve surface conductivity. The oxidative coupling can be performed in the presence of FeCl 3 (A) or with a mixture of FeCl 3 and EDOT (B). When the oxidative coupling is performed with dissolved TH-38, insoluble particles precipitate due to uncontrolled crosslinking (C). should bridge the distance between the thiophene groups on the crystal surface (Scheme 2C). By copolymerization with EDOT as the linker between the thiophenes conductive behavior on the crystal surface should be feasible. Also during the copolymerization special care was taken that the TH-38 nanoplatelets were not destroyed, which was proven by TEM imaging after the polymerization (Fig. 3B right). From the TEM images only nanoplatelets were observed without any additional visible impurities, indicating the successful copolymerization on the surface on the crystals. In addition, the sample proved a substantial increase in conductivity, with a current level of 2.7 × 10 −9 A at 1 V and 4.7 × 10 −7 A at 20 V. Thus, it is likely that EDOT copolymerized with the thio-phene groups "on surface" (Fig. 3C right). As shown in Fig. S11, † the current level was linearly proportional to the applied voltages in the low bias regime, revealing the Ohmic nature of conduction through the poly(EDOT-co-TH-38) surface layer. 17 Observation of an Ohmic behavior is indicative of good contact formation between the Au electrodes and the thiophene-EDOT surface of the 2D conductive crystals. Besides the desired copolymerization between the thiophene groups of TH-38 and EDOT, also the homopolymerization of EDOT to form poly(3,4-ethylenedioxythiophene (PEDOT) might occur. After the polymerization, the crystals were purified by centrifugation to remove FeCl 3 and PEDOT, which might have formed as a side product. Then, the platelets were visualized by TEM   (Fig. 3B); from the TEM imaging, no additional polymer nanoparticles or aggregates could be visualized, which hints that no homopolymer was present after workup. Moreover, no FeCl 3 residues were found during TEM examination. These would be visible as small dark spots in the TEM micrographs. In addition, DSC measurements did not show signs of PEDOT (Fig. 3D). In order to prove that the observed conductivity resulted from the formation of bonds between thiophene groups in the polymer chain and EDOT, but not only due to formation of PEDOT, which might even not be detectable by DSC measurements, we performed a control experiment with polymer nanoplatelets carrying no thiophene groups. We prepared similar nanoplatelets using a long-chain polyphosphoester. 18 This polyethylene-like polymer carries 20 methylene groups between phosphate units and our previous findings proved that they form very similar nanoplatelets when crystallized from a dilute solution. The nanoplatelets were prepared accordingly and EDOT and FeCl 3 were added to initiate the polymerization. As the phosphate units cannot generate a copolymer with EDOT only homopolymerization is possible.

Polymer Chemistry Paper
After the reaction, we purified the nanoplatelets in the same way and measured their conductivity but, importantly, we did not observe an increased conductivity (Fig. S12 †). Together, these experiments prove that we were able to prepare 2D nanoplatelets from polyethylene-like polymers carrying thiophene units on their surface and that conductivity on the crystal surface was achieved by copolymerization with EDOT in dispersion.

Conclusion and outlook
We demonstrated a new method to generate polymer 2D lamellar nanoplatelets with a conductive surface. By crystallizing polyethylene-derivatives from a dilute solution that carry thiophene groups with a precise, equidistant distribution along their backbone, lamellar crystals with a constant thickness and a thiophene surface functionalization were obtained (nanoplatelets). The thiophene groups, expelled from the crystal surface, were copolymerized with EDOT, yielding a conductive surface. This is a new, versatile concept exploiting the crystallization of a polyethylene-derivative with build-in in-chain functional groups to spatially control conductivity on the surface of nanoplatelets. Because the crystallization from solution can be easily controlled, a combination of polymers, doped with different functional groups, can be co-crystallized and will yield a nanostructured polymer crystal with a local control of the chemical groups on the surface. Accordingly, this new method has the potential to serve as a versatile concept to achieve nanostructured surface functionalization, not only for microelectronic applications.

Author contributions
OS synthesized the polymers, conducted the investigations and wrote the original draft of the manuscript. BJ and KA per-formed and analyzed the conductivity measurements. KL supervised the project. FRW supervised the polymer synthesis and contributed to the concept of this work. IL developed the concept of this work and edited the manuscript.

Conflicts of interest
There are no conflicts to declare.